Plastic Deformation in Crystalline Materials Lecture 1 ... 1-Overview_1.pdf¢ Plastic...
Embed Size (px)
Transcript of Plastic Deformation in Crystalline Materials Lecture 1 ... 1-Overview_1.pdf¢ Plastic...
Plastic Deformation in Crystalline Materials
Kamyar Davoudi ���
Lecture 1: Overview
Structure of Solids
Quasi-crystalline* (ordered but not periodic; lacks translational symmetry)
• Solids are often crystalline. • A solid may be found in a crystalline or amorphous
form. Each may have its own applications��� For example:
• Crystalline silicon (Si) are used in ICs. • Amorphous silicon (Si) are sometimes used in Li-ion
batteries and solar cells • Amorphous metals are often called metallic glasses • It is really hard to make some metals amorphous (e.g.
Crystalline vs Amorphous Solids
Let’s start with some ��� ��� elementary diagrams ��� ��� we saw in elementary mechanics of materials and ask ��� ���
Some questions 4
Low carbon steel Aluminum Alloy
Stress-Strain Curve of a metal under uniaxial loading: ��� One of the first things we learned in mechanics of materials
• Why do materials become plastic? What is the mechanism of plastic deformation?
• Why stress-strain curves of different materials are different?
• How can we model strain hardening (= work hardening)?
Questions: [Beer & Johnston et al, mechanics of materials]
Stress-Strain Curve – Loading and Unloading
Again what we saw in the first chapters of mechanics of materials
[Beer & Johnston et al, mechanics of materials]
[Xiang, Vlassak, Acta Mater, 2006]
What causes the Bauschinger effect?
Effects of Orientation & Loading Rates���
m 2 ]
Nominal Shear [%]
Nominal stress strain curves (without correction for area changes and orientation changes) for 99.99% pure Al, at two tensile strain rates: three single crsytals of different orientations and one polycrystal of a grain size of 0.2 mm. After Kocks et al., Work Hardening, 1968
• How does the orientation affect the deformation?
• What is the difference between deformation of single crystal and polycrystal?
• How does the loading rate affect the deformation?��� ���
Effects of Temperature
Question: How does the temperature affect the hardening rate?
strain vs time (in tension) strain vs time (in compression)
Three stages: (I) primary creep regime (II) quasi-steady-state regime (III) tertiary creep regime
Question: What is the explanation for each regime?
Size Dependent Behavior: Experiment
Pure Ni microsamples having a orientation (A) stress-strain curves for samples with different diameters (B) SEM image at 4% strain (diameter 20 µm) (C) SEM image at 19% strain (diameter 5 µm) [Uchic et al., Science, 2008]
Another Experiment: Bulge Test
• Applied pressure p and membrane deflection h are measured • Average stress and strain are determined using following (or more sophisticated)
, ε= ε0 + 2δ2 3a2
: residual strain in the film ε0
before pressure is applied after pressure is applied
[Xiang, Vlassak, Scripta Mater., 2005]
Plane Strain Model:
Bulge Test - II
σ"6 0o h
Effect of Film Thickness: Effect of Passivation:
Cu Films with both surfaces passivated of different film thicknesses
Cu film of thickness h = 340 nm
[Xiang, Vlassak, Acta Mater., 2006]
Importance of Study of Mechanical Behavior of Materials at Small Scales
Detailed and quantitative understanding of size effect is essential for a reliable design
Many of failure mechanisms are stress-driven
It is critical to know the strength of a component in a device and hence the level of stress it can support
1980s Small Scale Devices
Experiments exhibited size dependence1990s
1950s Hall – Petch effect Brenner’s paper on whiskers Conference in NY
1924 First Report by G.I. Taylor
Continuum Mechanics Approach for Size Effect
In classical approach:
In nonlocal approach
This requires introduction of one or more length parameters into the constitutive equation
There is no strain gradient theory that can be applied to all experiments
!σ= function( !ε, T,…)
!σ= function( !ε,∇ !ε, ∇ 2 !ε, …,T,…)
f(σij ,εij p ,k)= F(σij ,εij
p )−k2(εp e )= 0
“it is sometimes said that the turbulent flow of fluids is the most difficult remaining problem in classical physics. Not so. Work hardening is worse.” (A.H. Cottrell, 2002)
2 4 6 8 10
(Kocks, Trans ASME, 1970)
• We should consider why and how crystals deform plastically.
Ideal Shear Strength
Consider a single crystal
τ = τmax sin
If τ < τmax : shear strain is elastic and will disappear when the stress is released.
For very low value of γ = x / a : τ = G γ
dτ dγ ⎛
Gb 2πa ≈
More accurate calculations showed that τmax= G/30 which is still >>measured shear strength
Ideal shear strength >> measured shear strength
81 years ago : Dislocations
Why materials become plastic
G.I. Taylor Egon Orowan Michael Polyani
Work hardening was the first problem that was considered
16 volumes of “Dislocations in Solids”
1953 A.H. Cottrell: [Work hardening] was the first problem to be attempted by dislocation theory and may be the last to be solved
2009 L. Kubin: There is presently no generally accepted theory explaining how and why organized dislocation microstructures emerge during plastic flow
2003 U.F. Kocks & H. Mecking Work hardening is as hopeless as ever
Work hardening was the first problem that was considered
G.I. Taylor F. Nabarro
Frederick C Frank
Nevil Mott* Rudolf Peierls* William Schockley*
Alan Cottrell U Fred KocksJ. Friedel T Mura H. Mecking
John Hirth Jens Lothe J. & J. Weertman
Ladislas Kubin 22
* Nobel Laurites
Work Hardening Modeling
• Collective motion of dislocations è Plastic Deformation
• Individual processes are well understood • Understanding overall effects is challenging without
some main processes into the model ��� à Discrete Dislocation Dynamics
Discrete Dislocation Dynamics
Continuum Mechanics��� ���
Finite Element Method
Computational Quantum Mech.
DFT: 1968��� roots: Thomas-Fermi, 1927
Alder, Wainwright, 1951
R Courant, 1943 R Clough, coworkers: 1960
Amodeo, Ghoniem, 1990
Kubin, et al., 1992